# ductile iron pipe vs bccp pipe - articles/ آ ductile iron pipe versus bccp pipe 3 percent

Post on 18-Jan-2020

1 views

Embed Size (px)

TRANSCRIPT

DUCTILE IRON PIPE VERSUS BCCP PIPE

®

DUCTILE IRON PIPE VERSUS BCCP PIPE 1

A Comparison of Ductile Iron Pipe versus Bar-Wrapped Concrete Cylinder Pipe: All Pipe Materials are Not Equal

There’s a new substitute pipe on the block. Actually, it’s been around awhile but now has a new name. Still manufactured following the ANSI/AWWA C3031 standard, the former Pretensioned Concrete Cylinder pipe is now commonly referred to as “Bar-Wrapped Concrete Cylinder Pipe” (bccp). DIPRA, in its continuing effort to provide service to pipeline engineers and utilities, would like to point out just how bccp stacks up against Ductile Iron pipe.

As is usually the case when comparing Ductile Iron pipe with substitute materials, we find that all pipe materials are not

equal. Ductile Iron pipe’s conservative approaches and distinct advantages tip the scales decidedly in its favor.

Bccp is similar to steel pipe from the standpoint of internal pressure design, installation, corrosion control, field adaptability, pumping costs, and operation and maintenance requirements. Ductile Iron pipe’s many advantages along those lines will be explored in some detail and, when we conclude, we will have demonstrated why so many utilities and consulting engineers agree that Ductile Iron pipe is the right decision.

DUCTILE IRON PIPE VERSUS BCCP PIPE

L. Gregg Horn, P.E., DIPRA Director of Regional Engineers Allen H. Cox, P.E., DIPRA Senior Regional Engineer

2 DUCTILE IRON PIPE VERSUS BCCP PIPE

Ductile Iron Pipe Internal Pressure Design Is More Conservative The most important and interesting difference between Ductile Iron pipe and bccp is their design for internal pressure. A careful examination of these materials’ approaches to this important aspect of pipeline specification, while complicated by the composite nature of the concrete pipe, brings to light striking deficiencies in the bccp method.

Pipe wall thickness design in Ductile Iron pipe is a simple, yet conservative process. Ductile Iron pipe is a flexible conduit that is centrifugally cast from homogeneous molten Ductile Iron in accordance with the ANSI/AWWA C151/A21.51 standard “Ductile-Iron Pipe, Centrifugally Cast, for Water.”2

The pipe is designated as a “pressure class” product, which means that the wall thickness is calculated taking into account both working and surge pressures that the pipeline will experience. “Pressure Class 350” Ductile Iron pipe has a wall thickness that is calculated using a working pressure of 350 psi and an additional surge pressure of 100 psi with a nominal safety factor of 2.0, resulting in a design pressure of 900 psi.

The above description of the pressure class designation exemplifies the process for internal pressure design in the ANSI/AWWA C150/A21.50 standard “Thickness Design of Ductile-Iron Pipe.”3 In calculating the wall thickness required for internal pressure design, the Barlow Hoop Stress equation is used with the total working and surge pressures being applied against the minimum standard yield strength of Ductile Iron.

where:

t = Pipe wall thickness, inches Pw = Working pressure, psi Ps = Surge pressure, psi D = Pipe outside diameter, inches S = Stress in pipe wall, limited to the minimum tensile

yield strength of Ductile Iron, 42,000 psi

Examining the equation, we note that the nominal safety factor of 2.0 doubles the total pipeline pressure. Looking at it another way, this factor of safety limits the wall stress that develops from an internal pressure load to no more than 50 percent of the yield strength of Ductile Iron.

The inherent safety factor is increased in the design process by the addition of a “service allowance” to the wall thickness that results from the internal pressure calculation. The service allowance is a nominal 0.08-inch increase in wall thickness for all diameters and all classes of pipe. Completing the design, an allowance for casting tolerances is added. The size of the allowance is a function of the diameter of the pipe, as follows:

Nominal Pipe Size, inches Casting Allowance, inches 3 - 8 0.05

10 - 12 0.06 14 - 42 0.07

48 0.08 54 - 64 0.09

The allowance for the casting tolerance ensures that the wall thickness of the manufactured pipe is greater than the thickness required to sustain the design load. Thus, the casting process cannot compromise the factor of safety used in the design procedure. Further, due to the addition of the service allowance, the inherent safety factor will never be as low as the nominal safety factor of 2.0, even when maximum working plus surge pressures are considered.

Bar-Wrapped Concrete Cylinder Pipe Bccp is a composite product that is manufactured under the ANSI/AWWA C303 standard “Concrete Pressure Pipe, Bar- Wrapped, Steel-Cylinder Type.” It is classified by the concrete pipe industry as a “semi-rigid” pipe in that it does require ring deflection design for external load, but the limits of allowable deflection are very low to prevent cracking of the rigid protective cement-mortar coating. As with Ductile Iron pipe, separate stress analysis is employed wherein internal pressure and external loads are considered separately. The structural components are a cement-mortar-lined steel cylinder that is helically wrapped with a moderately tensioned round steel bar or wire and coated with, again, cement mortar (see Figure 1). The tension in the bars is simply enough, at least in theory, to ensure that internal pressure will engage both the cylinder and bar steel simultaneously. The cylinder and bar are used to sustain the internal pressure with the cylinder thickness and diameter and spacing of the bar wraps being variables. Jointing is accomplished through a bell and spigot configuration that is fabricated by welding joint rings to the cylinder. For purposes of external load calculations, all components of the pipe are considered bonded as a single unit and, therefore, a composite moment of inertia is used.

Figure 1: bccp Joint

General design considerations are discussed in ANSI/AWWA C303 and a more explicit procedure may be found in AWWA M9, “Manual of Water Supply Practices for Concrete Pressure Pipe,”4 which is referenced in the manufacturing standard. As with Ductile Iron pipe design, the Barlow Hoop Stress equation is used, although in a form that addresses the area of steel required (for both cylinder and bar wraps) per linear foot. Further, instead of using a factor of safety that is applied to the internal pressure, a “design factor” is applied to the allowable stress in the steel. The design procedure for bccp calls for limiting the allowable stress in the steel to 50

t = 2.0(Pw+Ps)(D)

2S

DUCTILE IRON PIPE VERSUS BCCP PIPE 3

percent (Design Factor=0.5) of the tensile yield strength when designing for working pressure, Pw, but allows the stress to go as high as 75 percent of yield when surge pressures are included. This is not a conservative approach because, unlike Ductile Iron pipe design, it allows a nominal safety factor as low as 1.33 under surge conditions. For working pressure design, the following equation is used:

where:

As = Area of steel, cylinder plus bar reinforcement, per linear foot

Pw = Working pressure, psi Dyi = Cylinder inside diameter, inches fs = Allowable stress, 50% of tensile yield strength

of steel, psi

For working pressure plus surge design, the following equation is used:

Where: Ps = Surge pressure, psi fst = Allowable stress for transient pressure, 75% of tensile

yield strength of steel, psi

Other Design Considerations

Other design considerations are discussed in ANSI/AWWA C303.5 There is an upper limit set for the steel in the bar reinforcement to be no more than 60 percent of the total steel area (cylinder and bar). Further, the bar area (in.2) per linear foot must be greater than or equal to 1 percent of the inside diameter of the pipe (in.). The clear space between the bar wraps can be no less than the diameter of the bar used; the maximum center-to-center spacing can be no more than 2 inches; the area of bar reinforcement can be no less than 0.23 in.2 per linear foot; and the minimum bar size is established at 7/32 of an inch. The minimum nominal cylinder thickness is a function of the pipe diameter and varies from 16 gauge (0.06 in.) for 10- through 21-inch pipe to 10 gauge (0.135 in.) for 51- through 60-inch pipe.

Equivalent Design

There are several significant differences in the respective ways the Ductile Iron pipe and bccp industries approach design for internal pressure. For one, Ductile Iron pipe design uses the outside diameter of the pipe in the Barlow equation when calculating the required thickness of the pipe wall, while bccp design uses the inside diameter of the steel cylinder. This simple difference is just one example of a design philosophy that results in a more conservative approach for Ductile Iron pipe compared to bccp. Other differences, which warrant more detailed discussion, include how surge pressures and material tolerances are addressed.

Surge Pressures

The most glaring difference between the design approaches of Ductile Iron and bccp is found in the way surge pressures are treated. As noted previously, Ductile Iron pipe applies a nominal safety factor of 2.0 to both the working and surge pressures (normally 100 psi), while bccp applies the same 2.0 safety factor (Design Factor=0.5) only to the working pressure. Surge pressures are allowed to increase the tensile stress in the cylinder and the bar wrap to as high as 75 percent of the yield strength of t